1. International Refereed Journal of Engineering and Science (IRJES)ISSN (Online) 2319-183X, (Print) 2319-1821Volume 2, Issue 4(April 2013), PP.11-16www.irjes.comwww.irjes.com 11 | PageMechanical Properties And Kinetics Of Weight Loss OfPolypropylene Waste Plastic Within The Very Low Extent OfWeight Loss Under Iso-Thermal Conditions.L.P.S Rohitha1, S.S.N. Perera2, M.A.B Prashantha31(Department of Earth Resources Engineering / University of Moratuwa, Sri Lanka)2(Research & Development Centre for Mathematical Modeling, Department of Mathematics,/ University ofColombo, Sri Lanka)3(Department of Chemistry / University of Sri Jayewardenepura, Sri Lanka)ABSTRACT: Polypropylene is one of the main raw materials used in plastic industry of Sri Lanka formanufacturing domestic plastic products. This paper was focused to study weigh loss of polypropyleneisothermal degradation, it’s mechanical properties, obtained order of reaction and as well as toughnessvariation at different temperature. However very low extent of weight loss (0.3% by mass) at iso-thermalconditions in the range of temperature 80 ˚C to 140 ˚C has significantly affected to the tensile strength,breaking strength, strain at break, and yield strength due to the evaporation of more volatile substances. It wasobserved variation of order of reaction at different temperature.Keywords - Waste Polypropylene, Mechanical property, Kinetics of weight loss, Iso-thermal conditions.I. INTRODUCTIONPolypropylene is one of the most important commercial polymers used in manufacture of a range of plasticproducts. In Sri Lanka, it is used in manufacturing the plastic furniture and range of plastic products fordomestic applications. Custom data of the last ten years indicates growth pattern of polypropylene based plasticmanufacturing industry in Sri Lanka . Recycling of plastics has become a small scale industry as a solutionfor the accumulation of plastics in the environment. The lowering of the physic-mechanical properties ofpolymer products is mainly due to the (a) decomposition of additives, (b) evaporation of volatile ingredients, (c)catalyst residues containing Ti, Al and Cl-, (d) unsaturated groups formed during polymerization by chaintransfer, or disproportionation of growing chain ends, and (e) carbonyl groups, introduced by carbon monoxideimpurities in the monomer and through oxidation, (f) reactive forms of oxygen such as ozone (O3) which ispresent in the atmosphere and singlet oxygen (1O2) which can be produced inside the polymer by quenching ofUV excited species by ground-state oxygen (3O2), (g) cross-linking and chain scissions of polymer molecules.The change in physico-mechanical properties of polymer products is typically very slow process under thetropical climate condition. Additives are used to optimize the physico-mechanical properties, minimize thedegradation under the environmental conditions and during the processing due to heat and mechanical stress.The knowledge of the change in physico-mechanical properties of plastics with the kinetics of weight loss isimportant to estimate the level of physico-mechanical properties of plastic waste for the recycling process.The standard power law kinetics model has been used to study the thermal degradation of polymer. Theequation (1) given below is the typical power law of Arrhenius equation used in studying the kinetics ofpolymers degradation under the isothermal condition. It is a combination of the effect of temperature andcontent of material remained to react .----------(1)Parameters of the equation (1) which α is the relative mass loss of the polymer at a time t, n is the order orpower of the kinetic equation, T is the absolute temperature, R is the gas constant, A is the pre-exponential factorand E is the activation energy. In the equation (2) the parameter W0 is the initial mass, Wt is mass at time t andWf is mass of sample at the end of experiment. The rate constant k is a product of A and exponential of -E/RT inArrhenius equation, k =.---------------(2)
2. Mechanical Properties And Kinetics Of Weight Loss Of Polypropylene Waste Plastic Within The Verywww.irjes.com 12 | PageKissinger, Fridman and Ozawa are the other proposed models used for evaluating the activation energy and pre-exponential factor in Arrhenius equation for the kinetics of polymer degradation . Number of alternativemodels proposed in literature are infinite Number of Parallel Reactions Model, the Weak Bond Model,Consecutive Reaction Models and, Simha and Wall Model. The complexity in practical applications of thesemodels was reviewed by R. W. J. Westerhout and et al . However, the simplicity of power model to use inpractical purpose is the main advantage.A first order kinetic equation has been used in most of literature to study the thermal degradation of polymer.The literature values of activation energy and frequency factor of degradation kinetics of polypropylene indicatethe inconsistency [4-9]. Thermo-gravimetric analysis (TGA) under the isothermal and non-isothermal conditionis a common technique to study the kinetics of polymer degradations. The degradation kinetic under isothermalconditions is preferred since the interpretation of data is simple and one parameter (conversion α) is monitoredduring an experiment, instead of two parameters, α and T, in the case of non-isothermal methods. Huimin Wangetal  has shown the change in the activation energy during the entire degradation process of polymer.Change in activation energy of degradation suggests a sequence of reactions and demonstrate complex kineticsof polymer degradation. Chemical structures of polymer molecule are stable below the 100 oC temperatureand usually stable 100 oC - 200 oC range. However, degradation is very prominent at 400 oC to 600 oC sincethe thermal energy at that temperature range is sufficient for energy requirement of bond breaking which have150- 400 kg mol-1.Degradation of plastics and activation energies of reactions during the degradation were studied at highertemperature above 200 oC. The attention of change in mechanical and spectroscopic properties prolongexposure to the temperature around the 100 oC is very rare. Loss of these organic additives such as stabilizersand plasticizers in the matrix will significantly affect to inferior quality of the physical and mechanicalproperties of commercial plastic before the real degradation of polymer molecules. The objective of thisresearch project is to study polypropylene waste plastic as a model plastic material to evaluate the change inmechanical properties, spectroscopic properties, with the kinetics of weight loss nearly up to 0.3% (as w/w%)under four different isothermal conditions at 80 oC ,100 oC,120 oC, 140 oC.II. MATERIAL AND METHODPolypropylene plastic boxes used in ice cream industry were selected in this study as a model material.Flat surface area of boxes with 0.2mm thickness was selected for dumbbell shaped test piece. Each set ofsamples were separately kept isothermal conditions at 80, 100, 120, 140 ˚C. At each time three pieces wereexamined for the measurements of weight loss, melt flow index (MFI), stress strain behavior and studied therelative changes in FTIR spectrums. In each set of three samples, average of measurements was used for theKinetics of weight loss and MFI. Integrated version of Arrhenius equation was used to analyze the kinetics ofweight loss within three different iso-conversional limits of α from 0.0 to 0.4, 0.4 to 0.6 and 0.6 to 0.9, .III. RESULTS AND DISCUSSIONTable 1 shows the variation of activation energy, pre-exponential factor, power of the kinetic equation, rateconstant and correlation coefficient (r2) in the range of α from zero to 0.4, 0.4 to 0.6 and 0.6 to 0.9 respectivelyat the four different isothermal conditions. Activation energy of the kinetics of weight loss at these four differenttemperature within the three different ranges of α was very low compared to the literature values (217 kj mol-1)reported for the degradation process at the temperature above 200 ˚C. The calculated values of pre-exponentialfactor at the four different isothermal conditions were also very low compared to the range 1.5 ×1012to 1.7 ×1012s-1K-0.5reported in the literature. Low activation energy and very low pre-exponential factor indicatephysical nature of the process during these four different isothermal conditions below 200 °C. Melt flow indexis an indication of average molar mass of polymer. The melt flow index of commercial PP samples is 4.3 g/10min. MFI of samples are not significantly changed even after 14 hours period of time under the differentisothermal conditions. It suggested that the 14 hours duration under the isothermal conditions was not sufficientfor the real degradation of polymer molecules.The activation energy has not significantly changed and nearly 26 KJ mol-1within the four different temperaturein the range of α from zero to 0.6. However, it has increased to 62 KJ mol-1 as α exceeds 0.6. It indicates theeffect of textural changes as a result of evaporation of volatile materials to increase the energy barrier for theevaporation of volatile substances or declining of easily volatile substance. Order of the kinetic equation haschanged from 2 to in the range of α from zero to 0.9 and these values agreed with the values in literature .Figure 1 shows the increasing pattern of power of kinetic equation in the range of α from 0.0 to 0.4 withtemperature. It is an indication of the linear relation between the textural changes with thermal expansion for theevaporation of easily volatile substances.
3. Mechanical Properties And Kinetics Of Weight Loss Of Polypropylene Waste Plastic Within The Verywww.irjes.com 13 | PageTable 1: Kinetic parameters at the four different temperature.Range of conversion α = 0.0 - 0.4Temperature 80 °C 100 °C 120 °C 140 °CE (KJ/ mol) 26.9 26.80 27.5 26.6A (min-1) 32.52 32.52 32.52 32.52r2 0.9772 0.9633 0.9921 0.9698n 2/5 6/5 7/5 2K (min-1) 3.5 × 10-35.8 ×10-37.2 × 10-31.4 ×10-2Range of conversion α = 0.4 - 0.6Temperature 80 °C 100 °C 120 °C 140 °CE (KJ/ mol) 26.06 25.0 25.5 26.0A (min-1) 12.90 12.90 12.90 12.90r20.9592 0.9632 0.9925 0.9839n 1/5 8/5 1 3/5K (min -1) 1.8 X10-34.1 X 10-35.2 X10-36.7 X 10-3Range of conversion α = 0 .6 - 0.9Temperature 80 °C 100 °C 120 °C 140 °CE (KJ/ mol) 62.35 61.24 62.91 61.80A (min-1) 3 × 10-43 × 10-4 3 × 10-4 3 × 10-4r20.9935 0.9197 0.9618 0.9877n 1/5 2/5 3/5 2/5K (min-1) 2.0 × 10-48.5 × 10-41.4 × 10-34.9 × 10-3However, such linear relation was not prominent as α exceeds 0.4. It indicated the complexity of the texturalchanges with decreasing the amount of more volatile substances and commencing the evaporation of lessvolatile substance as the magnitude of α exceeds 0.4. The magnitude of rate constant within the three ranges of αdecrease with the temperature as expected and Figure 2 shows the agreement between lnK and 1/T. Table 1indicates that the rate constant is also a function of α at a constant temperature. Rate constant has decreased withthe range of α from 0.0 - 0.4 to 0.6 - 0.9. This can be related to the net effect of declining of evaporation of morevolatile substances, textural changes due to the evaporation of substances from the texture and commencing ofthe evaporation of less volatile substances.Figure 1- Variation of the power of the kinetic equation with absolute temperatureFTIR spectrums (Figure 3 and 4) of polypropylene sample after 14 hours period of time under the isothermaltemperature at 80, 100, 120, 140 ˚C are almost same and comparable with original sample. It suggests that 14hours period of time at these isothermal conditions are not sufficient for chemical changes of molecules.
4. Mechanical Properties And Kinetics Of Weight Loss Of Polypropylene Waste Plastic Within The Verywww.irjes.com 14 | PageFigure 2- Variation of the lnK with the reciprocal value of absolute temperatureFigure 3- FTIR Spectrum of commercial PP before exposing to the thermal environmentTable 2 shows the effect of temperature on mechanical properties within the three different ranges of α.Mechanical properties of samples at 0.4 of α under the four different isothermal conditions are similar to theinitial properties of samples. However, mechanical properties have significantly changed as the conversionreaches to 0.9. Tensile strength, braking strength and yield strength has increased by 31%, 35% and 10%respectively and strain at brake has decreased by 40% under the isothermal condition at 80°C. Changes ofmechanical properties are significant even at law limit of α to the 0.3% of weight loss below 100 °C.
5. Mechanical Properties And Kinetics Of Weight Loss Of Polypropylene Waste Plastic Within The Verywww.irjes.com 15 | PageFigure 4- FTIR Spectrum of commercial PP after 14 hours at 140 °C.Braking strength has decreased by 65%, 70.6% and 89% under the isothermal condition at 100 °C, 120°C and140°C respectively. Weight loss due to the evaporation of more volatile substances has significantly increasedthe rigidity even at very low extent of weight loss.Table 2- Mechanical properties at different isothermal conditionsConversion α= 0.480°C 100°C 120°C 140°CTensile strength (MPa) 33.65 33.65 33.65 33.65Braking strength (MPa) 28.85 28.85 28.85 28.75Strain at brake 3.748 3.748 3.748 3.748Yield strength(MPa) Elastic Limit (0.2) 32.65 32.65 32.65 32.65Conversion α = 0.6Tensile strength (MPa) 41.5 43.15 54 48Braking strength (MPa) 36.85 37.35 50.62 48Strain at brake 3.08 3.04 1.71 0.6Yield strength(MPa) Elastic Limit (0.2) 36 36 46 46Conversion α= 0.99Tensile strength (MPa) 44 44 38 35.5Braking strength (MPa) 39 43.4 37 35.5Strain at brake 2.25 1.3 1.1 0.4Yield strength(MPa) Elastic Limit (0.2) 36 42 37.5 35.5
6. Mechanical Properties And Kinetics Of Weight Loss Of Polypropylene Waste Plastic Within The Verywww.irjes.com 16 | PageIV. CONCLUSIONKinetics of the weight loss of the waste polypropylene was studied under four different isothermalconditions. It was found 0.3%. Existing relationship in between activation energy and pre-exponential factor arefunction of the extent of conversion and temperature. Measurements of MFI and FTIR spectrums are notsignificantly change with the conversion of weight loss and hence change in weight loss is not mainly due to thedegradation of polymer molecules. Rigidity has increased due to the loss of plasticizing effect of polypropyleneproducts as a result of evaporation of more volatile substances. Even though small weight loss has led to highlychanged of mechanical properties of polypropylene.REFERENCES Sri Lanka Custom (2011), Import / Export data system, Sri Lanka Custom, Colombo.Available at:http://www.customs.gov.lk/stat.htm. Accessed 20 May 2011. Roy, P. K., Surekha, P., Rajagopal, C & Choudhary,V.(2007), Thermal degradation studies of LDPE containing cobaltstearate aspro-oxidant, eXPRESS Polymer Letters: l.1,(4):208–216 King, W. I, Kim, S.D., Lee, S.B & Hong, I.K.(2000), Kinetic Characterization of Thermal Degradation Process for CommercialRubbers, Journal of industrial and Engineering Chemistry 6(5):348-355 Westerhout, R. W. J., Waanders, J. , Kuipers, J. A. M & Swaaij, W. P. M. V. (1997), Kinetics of the Low-Temperature Pyrolysis ofPolyethene, Polypropene, and Polystyrene, Modeling, Experimental Determination, and Comparison with Literature Models andData, Ind.Eng. Chem. Res:36:1955-1964. Westerhout, R. W. J., Balk, R. H. P., Meijer, R., Kuipers, J. A. M., & Swaaij, W. P. M.V.(1997) Examination and Evaluation of theUse of Screen Heaters for the Measurement of the High Temperature Pyrolysis Kinetics of Polyethene and PolypropeneInd. Eng.Chem. Res.:36: 3360-3368. Peterson, D.J.,Vyazovkin, S., Wight, C.A,(2001)., Kinetics of the Thermal and Thermo-Oxidative Degradation of Polystyrene,Polyethylene and Poly(propylene). Macromol. Chem. Phys.: 202: 775–784. Westerhout, R. W. J., Waanders, J., Kuipers, J. A. M & Swaaij, W. P.M.V. (1997). Kinetics of the Low-Temperature Pyrolysis ofPolyethene, Polypropene, and Polystyrene, Modeling, Experimental, Determination, and Comparison with Literature Models andData Ind. Eng. Chem. Res. 1997, 36, 1955. Chien, J. C. W. & Kiang, J. K. Y.(1980). Macromolecules: 1980, 13,280. J. H. Chan, S. T. Balke, (1997).The thermal degradation kinetics of polypropylene: PartIII. Thermo gravimetric analyses, Polym.Degrad. Stabil: 57:135. Wang, H., Tao, X Newton, E. ( 2004)., Thermal degradation kinetics and lifetime prediction of a luminescent conducting polymer,Polym Int: 53:20–26. P. A. Dilara1*; D. Briassoulis,(2000), Degradation and Stabilization of Low-density Polyethylene Films used as Greenhouse, J. agric.Engng Res: 76, 309-321. Vyazoykin,S.,Dranca,I.,Fan,X.,Advincula,R.(2004), Kinetic of the thermal and thermo-Oxidative Degradation of a polystyrene-ClayNanocomposite, Macromolecular Rapid Communication: 25: 498-503. Kim, T. H., & Oh, S.C.(2005)., Kinetics of Thermal Degradation of Waste Polystyrene and High-Density, Polyethylene.J.Ind.Eng.Chem: 11(5):648-656,